Xianyuan Fan 1,2, Hong Liu 1,2,*, Emmanuella Anang 1 and Dajun Ren 1,2
1 Department of Resource and Environmental Engineering, Wuhan University of Science and Technology, Wuhan 430081, China; [email protected] (X.F.); [email protected] (E.A.); [email protected] (D.R.) 2 Hubei Key Laboratory for Efﬁcient Utilization and Agglomeration of Metallurgic Mineral Resources, Wuhan University of Science and Technology, Wuhan 430081, China * Correspondence: [email protected]; Tel.: +86-139-7148-8669
Abstract: The adsorption capacity of synthetic NaX zeolite for Pb2+, Cd2+, Cu2+ and Zn2+ in single and multi-component systems were investigated. The effects of electronegativity and hydration energy on the selective adsorption, as well as potential selective adsorption mechanism of the NaX zeolite for Pb2+, Cd2+, Cu2+ and Zn2+ were also discussed. The maximum adsorption capacity order of the heavy metals in the single system was Pb2+ > Cd2+ > Cu2+ > Zn2+, and this could be related to their hydration energy and electronegativity. The values of the separation factors (α) and afﬁnity 2+ 2+ constant (KEL) in different binary systems indicated that Pb was preferentially adsorbed, and Zn presented the lowest afﬁnity for NaX zeolite. The selective adsorption capacities of the metals were in 2+ 2+ 2+ 2+ Citation: Fan, X.; Liu, H.; Anang, E.; the order, Pb > Cd ≈ Cu > Zn . The trend for the selective adsorption of NaX zeolite in ternary Ren, D. Effects of Electronegativity and quaternary systems was consistent with that in the binary systems. Pb2+ and Cu2+ reduced the and Hydration Energy on the stability of the Si-O-Al bonds and the double six-membered rings in the NaX framework, due to the Selective Adsorption of Heavy Metal high electronegativity of Pb2+ and Cu2+ than that of Al3+. The selective adsorption mechanism of Ions by Synthetic NaX Zeolite. NaX zeolite for the high electronegative metal ions could mainly result from the negatively charged Materials 2021, 14, 4066. https:// O in the Si-O-Al structure of the NaX zeolite, hence heavy metal ions with high electronegativity doi.org/10.3390/ma14154066 display a strong afﬁnity for the electron cloud of the oxygen atoms in the Si-O-Al. This study could evaluate the application and efﬁciency of zeolite in separating and recovering certain metal ions from Academic Editors: Bruno industrial wastewater. De Gennaro, Barbara Liguori, Abner Colella and Domenico Caputo Keywords: NaX zeolite; selective adsorption; heavy metal ion; electronegativity; hydration energy
Received: 1 June 2021 Accepted: 17 July 2021 Published: 21 July 2021 1. Introduction Publisher’s Note: MDPI stays neutral Heavy metal ions such as Pb(II), Cr(VI), Cu(II), Zn(II), Hg(II) and Ni(II), are highly with regard to jurisdictional claims in toxic, carcinogenic, difﬁcult to degrade, and accumulate in living organisms when they published maps and institutional afﬁl- get into the food chain . Their presence in the ecosystem pose great danger to both iations. human and environmental health, thus, the removal of such toxic substances is of much interest to researchers. Many conventional and modern methods aimed at removing heavy metals from environmental media have been developed and adopted over the years. Among the various techniques for heavy metal removal in wastewater, such as chemical Copyright: © 2021 by the authors. precipitation, chemical reduction, ion-exchange, electrochemical treatment, reverse osmosis Licensee MDPI, Basel, Switzerland. and membrane technologies, adsorption is regarded as the simplest, most effective and This article is an open access article environmentally friendly remediation process [2,3]. distributed under the terms and Adsorption which denotes the attachment of a substance onto a surface could repre- conditions of the Creative Commons sent a feasible solution to ion exchange, and removal of heavy metals by natural or synthetic Attribution (CC BY) license (https:// substrates . Adsorbents, which may include clay, activated carbon, hydroxyapatite, resin creativecommons.org/licenses/by/ or chitosan, are essential components in the adsorption process, and are expected to have 4.0/).
Materials 2021, 14, 4066. https://doi.org/10.3390/ma14154066 https://www.mdpi.com/journal/materials Materials 2021, 14, 4066 2 of 16
high adsorption interactions with target contaminants in order to effectively remove them from wastewater [3,5,6]. Clay minerals, such as bentonite, zeolite and montmorillonite present several advantages including large speciﬁc surface areas, large ion-exchange capac- ities for heavy metal ions and widespread deposits [3,7–9]. However, selectivity for heavy metal ions, adsorption capacities and stability are relatively low in natural clay minerals, particularly, zeolites. In contrast, the adsorption capacities of synthetic zeolites are higher than those of natural zeolites due to their larger speciﬁc surface areas, controlled structural compositions, high thermal and chemical stability [10–12]. Therefore, synthetic zeolites display great potential for the treatment of wastewater containing heavy metals. Zeolite X is a three-dimensional crystal structure that is rich in synthetic Al. Its building blocks are made up of sodalite cells that are tetrahedrally interconnected at single six rings by bridging oxygen atoms to result in double six rings . Application and investigation of various synthetic zeolites to remove heavy metals from wastewater have been mainly focused on the adsorption of single heavy metal ions [11,14–17], with few studies that are considering selective ion adsorption in multi-component systems [18,19]. Industrial wastewater usually contains two or more metals, and the presence of coexisting ions in the solution will inevitably affect the adsorption capacity of the materials to target pollutants. When ions are present in binary or multiple aqueous solutions with regards to the combined impact of the different heavy metal ions and synthetic zeolites, the conclusion of selective adsorption between metals species is not quite consistent [20,21]. The [AlO4] tetrahedral units in the synthetic zeolites’ frameworks are negatively charged, and could be neutralized by alkali metal cations (Na+, Ca2+,K+) introduced during the synthetic process. The alkali metal cations can easily be exchanged because they are free within the zeolite frameworks [22–25]. The pore size of synthetic zeolites may be an important factor affecting their selective adsorption, particularly when the diameter of hydrated ions is larger, metal ions may be excluded. Dehydration facilitates the movement of ions into the zeolite channels [26,27]. Therefore, the selective adsorption of synthetic zeolites for heavy metal ions may be related to the diameter and hydration energy of the corresponding hydrated ion. A few studies [10,28–30] reported that heavy metal cations with low electronegativity can be easily replaced in aluminosilicate-based materials by others with higher electroneg- ativity. For example, Xu et al.  found that Pb2+ was adsorbed on synthetic cancrinite by replacing Cd2+, due to its high electronegativity, as compared to Cd2+. According to Chao et al. , both K+ and H+ were replaced by Pb2+ in Si-O-K and Si-O-H type aluminosilicates due to the high electronegativity of Pb2+, but the metal uptake capacity was the same. Therefore, the electronegativity of heavy metals may also affect the selective adsorption behavior of aluminosilicate-based materials. Research on this phenomenon is rather limited. The selective adsorption of different heavy metals on synthetic zeolites and the un- derlying mechanisms are essential for the proper application of synthetic zeolites in the removal of heavy metal ions. In the present study, NaX zeolites with high ion-exchange capacity were selected as model materials. Common pollutants present in industrial wastewater such as Pb2+, Cd2+, Cu2+ and Zn2+ were also selected. The adsorption per- formances of NaX zeolites for Pb2+, Cd2+, Cu2+ and Zn2+ in single and multi-component solutions were systematically examined. The effects of electronegativity and hydration energy of Pb2+, Cd2+, Cu2+ and Zn2+ on the selective adsorption of NaX zeolites were in- vestigated. Furthermore, structural properties of NaX zeolites were considered in order to determine the relationship between the mechanisms of selective adsorption with hydration energy and electronegativity.
2. Materials and Methods 2.1. Materials The NaX zeolite used in the present research was supplied by Nankai University Catalyst Co. Ltd. (Tianjin, China). All reagents, including cupric nitrate, lead nitrate, Materials 2021, 14, 4066 3 of 16
cadmium nitrate, zinc nitrate, sodium hydroxide, and nitric acid were of analytical reagent grade and purchased from Sinopharm Chemical Reagent Co. (Shanghai, China). The pH of the tested solution was adjusted to the desired value by adding diluted sodium hydroxide or nitric acid.
2.2. Adsorption Experiments 2.2.1. Adsorption Isotherms Adsorption equilibrium isotherms for single and multi-component systems containing Pb2+, Cd2+, Cu2+, and Zn2+ were obtained at an optimum pH of 5 and temperature, 298 K. Batch adsorption experiments were carried out in a 1.0 L beaker. A volume of 0.8 L of a single or multi metal solution and 0.80 g of NaX zeolite were placed in the beaker. Later, the mixture was stirred for 24 h using a rotating rate of 160 rpm until equilibrium was reached. In mono-component adsorption systems, the initial concentrations for Pb2+, Cd2+, Cu2+ and Zn2+ varied between 0.5 mmol/L and 5.0 mmol/L. In binary solutions, the target metal ion concentrations varied over the range of 1.0 to 4.0 mmol/L. In addition, concentrations of the interfering metal species were 1.0, 2.0, 3.0, and 4.0 mmol/L, respectively. In ternary and quaternary solutions, the equimolar concentrations of each heavy metal ion were 0.25, 0.5, 1.0, 2.0, 3.0 and 4.0 mmol/L. The concentrations of the metal ions in the residual aqueous phase were analyzed with a ﬂame atomic absorption spectrophotometer (novAA350, Analytikjena, Germany). The amount of metal adsorbed per unit mass of NaX zeolite was determined using Equation (1), V(C −C ) Q = 0 e (1) e m
where C0 and Ce are the initial and equilibrium metal concentrations (mmol/L), respec- tively; m is the mass of NaX (g); V is the volume of the solution (L); and Qe is the equilibrium adsorption capacity (mmol/g). The concentrations of Na+ in the residual aqueous phase of single systems were analyzed with an ion chromatograph (883, Vantone, Switzerland). The concentration of Na+ in 1.0 g/L NaX aqueous solution was taken as blank background.
2.2.2. Time Proﬁles of Competitive Adsorption Process in the Binary Systems Solutions containing single or binary ions at concentrations, 2.0 and 3.0 mmol/L, were mixed with NaX zeolites (solid concentration 1.0 g/L, total volume 0.8 L). In binary systems, a molar ratio of 1:1 was selected. Mixtures were adjusted at an initial pH of 5 and mechanically stirred at 160 rpm at a temperature of 298 K. 0.005 L aliquots were taken at the pre-settled time intervals and concentrations of the adsorbed ions were calculated using Equation (1).
2.3. Modeling of Metal Adsorption Adsorption isotherms in single systems were obtained using Langmuir and Freundlich models as presented in Equations (2) and (3),
KLQmCe Qe = (2) 1 + KLCe
1/n Qe= KfCe (3)
where Ce is the equilibrium concentration (mmol/L); Qe is the equilibrium adsorption capacity (mmol/g); KL is the afﬁnity parameter or Langmuir sorption constant (L/mmol), which reﬂects the sorption free energy; Qm is the capacity parameter (mmol/g); Kf and n are the Freundlich constant isotherm parameters. Materials 2021, 14, 4066 4 of 16
In binary systems, the selectivity of competitive adsorption was concentration depen- dent . The separation factor (an index of selectivity) is expressed in Equation (4):
1 Qe1×Ce2 α2 = (4) Qe2×Ce1 In order to evaluate the afﬁnity of NaX zeolite towards the heavy metal ions, the ad- sorption data of binary systems were simulated with the extended Langmuir model [32,33]. The extended Langmuir model is expressed as [8,31,34]:
QmaxKEL,iCe,i Qe,i = (5) 1 + KEL,iCe,i+KEL,jCe,j
where Qmax is the maximum capacity (mmol/g) and KEL,i is the afﬁnity parameter or Langmuir adsorption constant (L/mmol). The three-dimensional isotherm surfaces were generated using MATLAB 2014b, with a minimum value of the residual sum of squares (RSS) and the chi-squared (χ2) which could be deﬁned as: 2 RSS = ∑ Qe,exp−Qe,ﬁt (6) 2 Qe,exp−Qe,ﬁt χ2 = ∑ (7) Qe,ﬁt
2.4. Characterization Fourier transform infrared spectrometer (Vertex70, Bruker, Germany) was used to analyze functional groups present in the NaX zeolites loaded with heavy metal ions. The speciﬁc surface areas and pore parameters of materials were determined using N2 adsorption-desorption method by a speciﬁc surface area analyzer (Micromeritics ASAP 2020, Atlanta, GA, USA). The X-ray diffraction (XRD) measurements for NaX zeolites powders were conducted by an X-ray diffractometer (max-IIIA, Rigaku D, Japan). The morphologies of NaX zeolites were characterized by a scanning electron microscopy (SEM) (Nova 400 Nano, FEI, Hillsboro, OR, USA). The laser particle size analyzer (Mastersizer 2000, Melvin, UK) was used to determine particle size distribution
3. Results and Discussion 3.1. Characterizations of NaX Zeolites The elemental content of commercial NaX zeolite and the mole of Si/Al are shown in Table1. The mole of Si/Al was 1.35, and the exchangeable cations were mostly Na +. Based on the contents of K, Na, Mg and Ca, the divalent cation exchange capacity (CEC) was calculated to be 2.393 mmol/g in NaX zeolite.
Table 1. Element content of NaX zeolite (wt %).
Element Si Al Ca Mg K Na n(Si/Al) Mass percentage 18.18 12.94 0.07 0.07 0.04 10.65 1.35
The SEM image, XRD pattern, particle size distribution, N2 adsorption-desorption isotherms and pore size distribution (inset) of NaX zeolite are shown in Figure1. The commercial NaX zeolite exhibits a cubic crystal system of octahedron (Figure1a), and particle size distribution d (0.5) of 4.213 µm (Figure1c). It was found that NaX zeolite exhibits a narrow pore size distribution of 0.55–0.56 nm (Figure1d). The BET speciﬁc 2 −1 surface area was 712.7 m ·g , and the shape of N2 adsorption-desorption isotherms was typically characteristic of microporous materials. Materials 2021, 14, x FOR PEER REVIEW 5 of 18
Table 1. Element content of NaX zeolite (wt %). Materials 2021, 14, 4066 5 of 16 Element Si Al Ca Mg K Na n(Si/Al) Mass percentage 18.18 12.94 0.07 0.07 0.04 10.65 1.35
Figure 1. Characterization of NaX zeolite, SEM image (a), XRD pattern (b), particle size distribution (c), N2 adsorp- Figure 1. Characterization of NaX zeolite, SEM image (a), XRD pattern (b), particle size distribution (c), N2 adsorption- tion-desorption isotherms and Pore size distribution (inset) (d). desorption isotherms and Pore size distribution (inset) (d).
2+ 2+ 2+ 2+ 22.214.171.124. Adsorption Adsorption of Pb of Pb, Cd2+, Cd, Cu2+, Cuand2+ Znand by Zn NaX2+ by Zeolites NaX Zeolites in a Single ina System Single System In order to evaluate the adsorption capacity of NaX for different heavy metals, Pb2+, In order to evaluate the adsorption capacity of NaX for different heavy metals, Pb2+, Cd2+, Cu2+ and Zn2+ were selected for adsorption experiments in a single system. The Cd2+, Cu2+ and Zn2+ were selected for adsorption experiments in a single system. The nonlinear isothermal fittings and fitting parameters are shown in Figure 2a and Table 2. nonlinear isothermal ﬁttings and ﬁtting parameters are shown in Figure2a and Table2. The results indicated that the Langmuir model justified the experimental data with an adequate correlation coefficient (R2 > 0.9), and the corresponding equilibrium adsorp- Table 2. Isotherm parameters for Pb2+, Cd2+, Cu2+ and Zn2+ sorption using NaX. tion capacity was 2.38, 2.14, 1.87 and 1.68 mmol/g for Pb2+, Cd2+, Cu2+ and Zn2+, respec- 2+ 2+ 2+ tively. The overall trend of adsorptionLangmuir capacity was in the order of Pb Freundlich > Cd > Cu > 2+ Zn .Metal Ions 2 2 Qm (mmol/g) KL (L/mmol) R Kf (mmol/g) n R The maximum adsorbed amounts of heavy metal ion (M2+) expressed as % of the 2+ divalentPb cation exchange2.375 capacity (CEC) 494.793 of NaX zeolites 0.9881 were calculated 2.3339 using 8.6640 Equation 0.7878 Cd2+ 2.144 95.720 0.9625 2.0242 7.3697 0.7999 2+ (8), andCu the2+ results are shown1.868 in Figure 134.795 2b. The results 0.9390 indicated 1.7668 that Pb could 7.7328 exchange 0.8321 almost Znall2+ exchangeable1.680 ions in NaX zeolites: 126.478 0.9017 1.5807 7.8530 0.9168
Q CEC(M2+) (%)= m ×100%. (8) The results indicated that the Langmuir modelCEC justiﬁed the experimental data with an adequate correlation coefﬁcient (R2 > 0.9), and the corresponding equilibrium adsorption capacity was 2.38, 2.14, 1.87 and 1.68 mmol/g for Pb2+, Cd2+, Cu2+ and Zn2+, respectively. The overall trend of adsorption capacity was in the order of Pb2+ > Cd2+ > Cu2+ > Zn2+.
Materials 2021, 14, x FOR PEER REVIEW 6 of 18
The ratio of adsorbed heavy metal ion (M2+) to exchanged Na+ are shown in Figure 2c. The individual R values for the heavy metals were scattered around 0.5 (Figure 2c), thus indicating that the removal of heavy metal ions may be attributed to their exchange with Na+ ions present in the NaX matrix. Compared to the size of the supercage in NaX (0.74–0.78 nm), the hydration diameter of the heavy metals (Pb2+ (0.802 nm), Cd2+ (0.852 nm), Cu2+ (0.838 nm), and Zn2+ (0.860 nm)) are just a little large. Therefore, heavy metal ions were able to enter the supercage of NaX and exchange with Na+. Some of the hydra- tion water was stripped from the solvated ions (dehydration). However, the exchange may rather be difficult because the cations are too big to diffuse through the 6-membered rings of the cubooctahedra and hexagonal prisms. The Pb2+ may lose all its hydration water to diffuse through the 6-membered rings (0.28 nm), but the others (Cd2+, Cu2+ or Zn2+) may not. Therefore Cd2+, Cu2+ or Zn2+ undergo partial exchange. Dehydration depends on the hydration energy of the corresponding metal ions, because the lower the hydration energy, the easier it is for the metal ion to dehydrate. The order of the hydration energy for the heavy metal ions was Pb2+ (1502 KJ/mol) < Cd2+ (1828 KJ/mol) < Zn2+ (2058 KJ/mol) < Cu2+ (2121 KJ/mol) . Pb2+ displayed the least hy- dration energy as compared to the other ions, thus hydrated Pb2+ can be easily dehy- drated. Hence, NaX displayed more adsorption capacity for Pb2+, as compared to the rest of the heavy metal ions. Similarly, Cd2+ adsorption can be explained by the same rule. However, the adsorption capacity of Zn2+ and Cu2+ displayed cannot be due to the rule of hydration energy, while Selim  and Liu  obtained the similar phenomenon. This result could be related to Pauling electronegativity and hydrated ionic radius of Cu2+ and Zn2+ . The hydration radius of hydrated Cu2+ is smaller than that of Zn2+. A larger hydrated radius means that the cationic center of charge is farther from the clay surface so the clay-cation electrostatic interaction is weaker . Moreover, Pauling electronega- Materials 2021, 14, 4066 tivity of copper (1.9) is higher than that of zinc (1.65) . Therefore, Cu2+ exhibited6 of 16a greater affinity towards the NaX.
99.3 2.5 (a) 100 (b) 89.6
80 78.1 2.0 70.2
1.5 2+ ) (%)
Q 2+ 40 1.0 Cu 2+ Zn CEC(M Langmuir fitting 20 0.5 Freundlich fitting Materials 2021, 14, x FOR PEER REVIEW 7 of 18
0.00.51.01.52.02.53.03.5 0 Pb Cu Zn Ce(mmol/L) Cd 0.6 (c) 0.5
0.4 Pb 0.3 Cd
R Cu 2+ Zn adsorbed [M ] 0.2 R= exchanged [Na+] 0.1
0.0 12345 C (mmol/L) 0
2+ 2+ 2+ 2+ 2+ Figure 2. ((a)) NaXNaX adsorptionadsorption isotherms isotherms for for Pb Pb2+,, CdCd2+, CuCu2+ andand Zn Zn2+; ;((bb) )the the M M2+ amountsamounts adsorbed adsorbed as as % % of of the the CEC; and ((c)) thethe ratioratio (R)(R) ofof adsorbedadsorbed [M[M2+2+]] to to exchanged exchanged [Na [Na++] ]during during the the adsorption adsorption process. process.
2+ Table 2. IsothermThe maximum parameters adsorbed for Pb2+, Cd amounts2+, Cu2+ and of Zn heavy2+ sorption metal using ion (MNaX. ) expressed as % of the divalent cation exchange capacity (CEC) of NaX zeolites were calculated using Equation (8), Langmuir Freundlich2+ Metal Ions and the results are shown in Figure2b. The results indicated that Pb could exchange Qm (mmol/g)almost all exchangeable KL (L/mmol) ions in NaX zeolites: R2 Kf (mmol/g) n R2 Pb2+ 2.375 494.793 0.9881 2.3339 8.6640 0.7878 + Q Cd2+ 2.144 95.720 CEC(M0.96252 ) ( %) = m2.0242×100%. 7.3697 0.7999 (8) Cu2+ 1.868 134.795 0.9390 CEC1.7668 7.7328 0.8321 Zn2+ 1.680 The ratio of adsorbed126.478 heavy metal0.9017 ion (M2+) to1.5807 exchanged Na+7.8530are shown in0.9168Figure 2c . The individual R values for the heavy metals were scattered around 0.5 (Figure2c ), thus 3.3.indicating Selective that Adsorption the removal of Target of Heavy heavy Metals metal in ions Binary may Systems be attributed by NaX Zeolites to their exchange withIn Na order+ ions to presentinvestigate in the the NaX effects matrix. of hydr Comparedation energy to theand sizeelectronegativity of the supercage on the in 2+ 2+ selectiveNaX (0.74–0.78 adsorption nm), of the Pb hydration2+, Cd2+, Cu diameter2+ and Zn of2+ using the heavy NaX, metals the following (Pb (0.802 binary nm), solution Cd 2+ 2+ systems(0.852 nm), were Cu designed:(0.838 nm), Cu2+ and-Pb2+ Zn, Cu2+(0.860-Cd2+, nm))Cu2+-Zn are2+ just and a littleCd2+-Zn large.2+. The Therefore, orders heavyof hy- + drationmetal ions energy were and able electronegativity to enter the supercage of the he ofavy NaX metals and in exchange different with binary Na systems. Some are of shownthe hydration in Table water 3. was stripped from the solvated ions (dehydration). However, the exchange may rather be difﬁcult because the cations are too big to diffuse through the 2+ Table 3. The orders of6-membered hydration energy rings and of electronegativity the cubooctahedra of the and heavy hexagonal metals in prisms.different The binary Pb systems.may lose all its hydration water to diffuse through the 6-membered rings (0.28 nm), but the others (Cd2+, Hydration En-2+ 2+ Heavy 2+ 2+ Pauling2+ Hydration Energy Binary Systems Cu orElectronegativity Zn ) may not. Therefore Cd , Cu or Zn undergo partial exchange. ergy Dehydration depends onMetals the hydration Electronegativity energy of the corresponding (KJ/mol) metal ions, be- Cu2+-Pb2+ Cu2+ > Pb2+cause the lowerCu2+ < thePb2+ hydration energy,Pb2+ the easier it2.33 is for the metal ion to dehydrate. 1502 The Cu2+-Cd2+ Cu2+ > Cd2+order of theCu hydration2+ > Cd2+ energy forCd2+ the heavy metal1.69 ions was Pb2+ (1502 KJ/mol) 1828 < Cd2+ Cu2+-Zn2+ Cu2+ > Zn2+(1828 KJ/mol)Cu2+ <> Zn2+ (2058 KJ/mol)Cu2+ < Cu2+ (21211.9 KJ/mol) . Pb2+ displayed 2121 the least Cd2+-Zn2+ Cd2+ < Zn2+ Cd2+ ≈ Zn2+ Zn2+ 1.65 2058
3.3.1. Binary Adsorption Equilibrium Isotherm Figure 3 shows adsorption isotherm and three-dimensional isotherm surfaces sim- ulated with the extended Langmuir isothermal model for the adsorption capacity of each metal set present in the four binary systems.
Materials 2021, 14, 4066 7 of 16
hydration energy as compared to the other ions, thus hydrated Pb2+ can be easily dehy- drated. Hence, NaX displayed more adsorption capacity for Pb2+, as compared to the rest of the heavy metal ions. Similarly, Cd2+ adsorption can be explained by the same rule. However, the adsorption capacity of Zn2+ and Cu2+ displayed cannot be due to the rule of hydration energy, while Selim  and Liu  obtained the similar phenomenon. This result could be related to Pauling electronegativity and hydrated ionic radius of Cu2+ and Zn2+ . The hydration radius of hydrated Cu2+ is smaller than that of Zn2+. A larger hydrated radius means that the cationic center of charge is farther from the clay surface so the clay-cation electrostatic interaction is weaker . Moreover, Pauling electronegativity of copper (1.9) is higher than that of zinc (1.65) . Therefore, Cu2+ exhibited a greater afﬁnity towards the NaX.
3.3. Selective Adsorption of Target Heavy Metals in Binary Systems by NaX Zeolites In order to investigate the effects of hydration energy and electronegativity on the selective adsorption of Pb2+, Cd2+, Cu2+ and Zn2+ using NaX, the following binary solution systems were designed: Cu2+-Pb2+, Cu2+-Cd2+, Cu2+-Zn2+ and Cd2+-Zn2+. The orders of hydration energy and electronegativity of the heavy metals in different binary systems are shown in Table3.
Table 3. The orders of hydration energy and electronegativity of the heavy metals in different binary systems.
Binary Systems Hydration Energy Electronegativity Heavy Metals Pauling Electronegativity Hydration Energy (KJ/mol) Cu2+-Pb2+ Cu2+ > Pb2+ Cu2+ < Pb2+ Pb2+ 2.33 1502 Cu2+-Cd2+ Cu2+ > Cd2+ Cu2+ > Cd2+ Cd2+ 1.69 1828 Cu2+-Zn2+ Cu2+ > Zn2+ Cu2+ > Zn2+ Cu2+ 1.9 2121 Cd2+-Zn2+ Cd2+ < Zn2+ Cd2+ ≈ Zn2+ Zn2+ 1.65 2058
3.3.1. Binary Adsorption Equilibrium Isotherm Figure3 shows adsorption isotherm and three-dimensional isotherm surfaces simu- lated with the extended Langmuir isothermal model for the adsorption capacity of each metal set present in the four binary systems.
Cu2+-Pb2+ Binary System In the Cu2+-Pb2+ binary system, Cu2+ served as the target ion, while Pb2+ was selected as the competitive ion during the process of Cu2+ adsorption. The Cu2+ adsorption surface isotherm displayed a concave downwards shape, but Pb2+ was closer to the XY plane par- ticularly at low initial concentrations (Figure3a). The adsorption capacity of Pb 2+ gradually increased to 2.3~2.4 mmol/g with increasing initial Pb2+ concentration (Figure3b ). The maximum capacity of Pb2+ was almost equal to that of Pb2+ in a single solute (Figure2 ). NaX will preferentially adsorb Pb2+, which displays lower hydration energy and higher electronegativity than Cu2+, and Cu2+ will be adsorbed only when the concentration of Pb2+ is insufﬁcient for NaX to reach adsorption saturation.
Cu2+-Cd2+ Binary System In the Cu2+-Cd2+ binary system, Cu2+ was selected as the target ion, while Cd2+ was selected as the competing ion. The adsorption capacity of Cu2+ increased with increasing Cu2+ concentrations but decreased when the Cd2+ concentration increased. The same effect was exhibited by the Cd2+ in the binary system (Figure3c,d), but Cu 2+ adsorption capacity gradually decreased to 0.92 mmol/g and Cd2+ adsorption capacity decreased to 0.93 mmol/g (when initial concentration C0,Cd = 4.0 mmol/L and C0,Cu = 4.0 mmol/L). It can be established that the NaX displayed similar selective adsorption behaviour with Cu2+ and Cd2+ even though the hydration energy of Cd2+ was smaller and more easily adsorbed, and the electronegativity of Cu2+ (1.9) was higher than Cd2+ (1.69). Materials 2021, 14, 4066 8 of 16 Materials 2021, 14, x FOR PEER REVIEW 8 of 18
Figure 3. AdsorptionAdsorption capacity of heavyheavy metalsmetals byby NaXNaX zeolitezeolite andand three-dimensionalthree-dimensional isothermisotherm surfacessurfaces simulatedsimulated withwith the extendedthe extended Langmuir Langmuir isotherm isotherm model: model: Cu2+-Pb Cu2+2+ binary-Pb2+ systembinary system(a,b), Cu (a2+,-Cdb), Cu2+ binary2+-Cd 2+systembinary (c,d system), Cu2+-Zn (c,d2+), binary Cu2+-Zn system2+ binary (e,f) and 2+ 2+ Cdsystem-Zn (e binary,f) and system Cd2+-Zn (g2+,h).binary system (g,h).
Materials 2021, 14, 4066 9 of 16
Cu2+-Zn2+ Binary System The adsorption capacity of Cu2+ (the target ion) was insigniﬁcantly affected by Zn2+ (the competing ion), thus, gradually increasing as Cu2+ concentration increased (Figure3e ) while Zn2+ decreased (Figure3f). When the concentration of Cu 2+ was set at 4.0 mmol/L and initial Zn2+ concentration increased, the adsorption capacity of Cu2+ decreased from 1.84 mmol/g to 1.41 mmol/g. The adsorption capacity of Zn2+ was only between 0.03 mmol/g and 0.26 mmol/g. NaX, thus, displayed better selective adsorp- tion performance for Cu2+ which presents relatively high electronegativity and similar hydration energy with Zn2+ in the Cu2+-Zn2+ binary system.
Cd2+-Zn2+ Binary System In the Cd2+-Zn2+ binary system, Zn2+ acted as the target ion, and Cd2+ as the com- peting ion. As shown in Figure3g,h, the adsorption capacity of Zn 2+ increased with increasing initial Zn2+ concentration. However, it gradually decreased until reaching a value of 0.80 mmol/g with increasing Cd2+ concentrations, and the adsorption ca- pacity of Cd2+decreased to 1.40 mmol/g with increasing Zn2+ concentrations (when 2+ CCd = 4.0 mmol/L, C0,Zn = 4.0 mmol/L). Since the electronegativity of Zn (1.65) is almost similar to that of Cd2+ (1.69) and Cd2+ demonstrated easy adsorption by the NaX zeolite due to its small hydration energy, the selectivity of NaX zeolite to Cd2+ was greater than Zn2+.
3.3.2. Afﬁnity Coefﬁcient (KEL) and Separation Factor (α) The simulated parameters of the extended Langmuir model, the maximum adsorption capacity Qmax and the afﬁnity coefﬁcient KEL are shown in Table4. The K EL value indicates 2+ 2+ the afﬁnity of the NaX zeolite towards the heavy metal ions. The KPb value in the Cu -Pb 2+ binary system was almost 119 times that of the KCu value. The afﬁnity of the NaX for Pb in the binary system was therefore higher than that for Cu2+. Moreover, in the Cu2+-Cd2+, 2+ 2+ 2+ 2+ Cu -Zn and Cd -Zn systems, the KEL ratio between the preferred ions (ions with high adsorption capacity) and the secondary species (ions with low adsorption capacity) were 1.15, 4.66, and 2.67 respectively. The afﬁnity of NaX zeolite towards Cu2+ and Cd2+ was similar, and that for Cu2+ was greater than Zn2+. In addition, the NaX afﬁnity for Cd2+ was slightly higher than Zn2+.
Table 4. Multi-component isotherm model parameters for the adsorption of Cu2+, Pb2+, Zn2+ and Cd2+ at 303 K.
2 Binary Systems Qmax (mmol/g) KEL (L/mmol) RSS χ 2+ 2+ Cu -Pb 2.416 KCu = 1.4391; KPb = 171.3544 2.3437 0.9701 2+ 2+ Cu -Cd 1.932 KCu = 91.5320; KCd = 94.0259 1.6519 0.8550 2+ 2+ Cu -Zn 1.851 KCu = 17.9153; KZn = 3.8476 0.9048 0.4888 2+ 2+ Cd -Zn 2.004 KCd = 21.5285; KZn = 8.0486 3.1121 1.5529
The separation factor, α, is an index of selectivity. The separation factors of the binary systems with equal molality ratio (1:1) obtained in this study are shown in Table5. Selected initial concentrations (C0) of each heavy metal ion in the binary systems were 1.0, 2.0, 3.0 Cu Cu Cu Cd and 4.0 mmol/L. When C0 was 1.0 mmol/L, the αPb , αCd, αZn and αZn separation factors were approximately equal to 1, thus, the heavy metal ions in the binary system are all Cu adsorbed when the NaX does not reach saturation. When C0 ≥ 2.0 mmol/L, the αPb value 2+ Cu was smaller than 1, indicative of the good selectivity of NaX towards Pb ; the αCd value was close to 1, indicating that the selectivity of NaX towards Cu2+ and Cd2+ was almost Cu Cd 2+ the same; the αZn and αZn values were greater than 1, indicating that NaX preferred Cu and Cd2+ over Zn2+. Materials 2021, 14, 4066 10 of 16
Table 5. Separation factors (α) in binary systems at equal molar ratios.
Cu Cu Cu Cd C0 (mmol/L) αPb αCd αZn αZn 1.0 0.9802 1.0000 1.0242 0.9968 2.0 0.0077 0.9533 4.7668 1.9258 3.0 0.0027 0.9609 4.9634 2.5103 4.0 0.0089 0.9860 11.5534 1.6304
3.3.3. Process of the Selective Adsorption in the Binary Systems The process of the selective adsorption for the Cu2+-Pb2+, Cu2+-Cd2+, Cu2+-Zn2+ and Cd2+-Zn2+ binary systems under equimolar concentrations are shown in Figure4. The adsorption capacity for Pb2+ in the binary system was consistent with that in the single system, but the adsorption capacity for Cu2+ signiﬁcantly reduced in the binary system. This was evident under both 2.0 and 3.0 mmol/L initial concentrations (Figure4a,b). Cu2+ adsorbed by the NaX was replaced by Pb2+ within 10 min when the Pb2+ amount superceded the adsorption capacity of NaX (Figure4b). Cu 2+ and Cd2+ demonstrated low adsorption capacity in the binary system under both 2.0 mmol/L and 3.0 mmol/L initial concentrations, but higher adsorption capacity in the single system (Figure4c,d). Adsorbed Cd2+ in the binary system was gradually replaced by Cu2+, which displays higher electronegativity. At the end of the process, the amounts of Cu2+ and Cd2+ adsorbed by the NaX were equivalent. In the Cu2+-Zn2+ binary system, Zn2+ adsorbed was gradually replaced by Cu2+, which is more electronegative than Zn2+ (Figure4e,f). The adsorption capacity of Zn2+ by the NaX varied signiﬁcantly, particularly in the 3 mmol/L initial concentration in both single and binary systems (Figure4f). Zn 2+ slowly decreased with increasing reaction time, while the adsorption capacity for Cd2+ did not show signiﬁcant changes (Figure4e,f). It is evident that Zn 2+ and Cd2+ did not replace each other in the Cd2+-Zn2+ binary system. Heavy metals that displayed small hydration energies were easier to dehydrate and subsequently be adsorbed by the NaX. However, in multiple ion systems, those ions with relatively high electronegativity were preferentially adsorbed by the NaX. Under 3.0 mmol/L initial concentration in the binary system, the molar masses of the ions ex- ceeded the maximum adsorption capacity per gram of zeolite. The results of the selective adsorption by NaX indicated that: (i) Pb2+, which displayed low hydration energy and high electronegativity as compared to Cu2+ was preferentially adsorbed until reaching the saturation in the NaX, while Cu2+ was not adsorbed (Figure4b); (ii) the adsorption capacity for Cu2+ with relatively high electronegativity was equivalent to that of Cd2+ which presented low hydration energy (Figure4d); (iii) in the Cu 2+-Zn2+ system, both elements presented similar hydration energies. Due to the higher electronegativity of Cu2+ as compared to Zn2+, the adsorption capacity for Cu2+ was more than three times that of Zn2+ (Figure4f ); (iv) Cd2+ and Zn2+ presented similar electronegativity values, while the adsorption capacity for Cd2+ which has low hydration energy, was only 1.8 times that of Zn2+ (Figure4h). Moreover, the adsorption capacity for Zn 2+ in the Cd2+-Zn2+ system was twice the one obtained for the Cu2+-Zn2+ system (Figure4f,h). Therefore, adsorption sites on the NaX were more likely bound to heavy metal ions that displayed higher electronegativity. The selective adsorption capacities of the metals were in the order Pb2+ > Cd2+≈Cu2+ > Zn2+.
3.4. Selective Adsorption of Heavy Metal Ions by NaX in Ternary and Quaternary Systems The NaX adsorption capacities for Pb2+, Cd2+, Cu2+ or Zn2+ in the ternary (Pb2+-Cd2+- Zn2+, Pb2+-Cd2+-Cu2+ and Cd2+-Cu2+-Zn2+) and quaternary systems (Pb2+-Cd2+-Cu2+- Zn2+) at equimolar concentrations are shown in Figure5. The results indicated that NaX was more selective towards Pb2+ than to the other three metals present in the multiple systems. Moreover, when the initial Pb2+ concentration was higher than 3.0 mmol/L, NaX did not adsorb other ions, hence, the adsorption capacity for Pb2+ was similar to that in the single system. The selective adsorption capacity of NaX for different heavy metal Materials 2021, 14, 4066 11 of 16
ions under the Pb2+-Cd2+-Zn2+, Pb2+-Cd2+-Cu2+, and Pb2+-Cd2+-Cu2+-Zn2+ systems was consistent with those observed in the binary systems (Figure5a,b,d). However, in the Materials 2021, 14, x FOR PEER REVIEW2+ 2+ 2+ 2+ 2+ 11 of 18 Cd -Cu -Zn group, when Cd and Cu concentrations were high enough to reach saturation in the NaX, Zn2+ adsorption was extremely low (Figure5c).
(a) 2.5 (b) 2.5 C0=2.0 mmol/L 2.0 2.0
1.5 single Pb2+ 1.5 C0=3.0 mmol/L 2+ binary Pb 2+ 1.0 2+ 1.0 Single Pb single Cu 2+ 2+ Binary Pb Q(mmol/g) Q(mmol/g) binary Cu 2+ 0.5 0.5 Single Cu 2+ Binary Cu 0.0 0.0 0 100 200 300 400 500 1300 1400 0 100 200 300 400 500 1300 1400 t(min) t(min) 2.5 (c) (d) 2.5 C0=2.0 mmol/L C 0=3.0 mmol/L 2.0 2.0
1.5 1.5 Q ＞ Q Q ≈ Q Q ＞ Q ≈ Cd Cu Cd Cu Cd Cu Q Cd Q Cu 1.0 1.0 Q(mmol/g) Q(mmol/g) 2+ 2+ 0.5 2+ 2+ 0.5 single Cd binary Cd single Cd binary Cd 2+ 2+ single Cu2+ binary Cu2+ single Cu binary Cu 0.0 0.0 0 100 200 300 400 1300 1400 0 100 200 300 400 1300 1400 t(min) t(min) 2.5 (f) 2.5 (e) C =3.0 mmol/L C 0=2.0 mmol/L 0 2.0 2.0
1.0 1.0 Q(mmol/g) Q(mmol/g) 0.5 2+ 2+ 0.5 2+ 2+ single Cu binary Cu single Cu binary Cu 2+ 2+ single Zn2+ binary Zn2+ single Zn binary Zn 0.0 0.0 0 200 400 600 1300 1400 0 200 400 600 1300 1400 t(min) t(min)
(g) 2.5 (h)2.5 C 0=2.0 mmol/L C 0=3.0 mmol/L 2.0 2.0
1.0 1.0 Q(mmol/g) Q(mmol/g) 2+ 2+ 0.5 2+ 2+ 0.5 single Cd binary Cd single Cd binary Cd 2+ 2+ 2+ 2+ single Zn binary Zn single Zn binary Zn 0.0 0.0 0 200 400 600 1300 1400 0 200 400 600 1300 1400 t(min) t(min) FigureFigure 4. Time 4. Time proﬁles profiles of heavy of heavy metals metals adsorption adsorption in in binary binary systemssystems using NaX NaX at at equal equal molar molar ratio: ratio: Cu2+ Cu-Pb2+2+-Pb binary2+ binary 2+ 2+ 2+ 2+ 2+ 2+ systemsystem (a,b), ( Cua,b2+), Cu-Cd-Cd2+ binary binary system system ( c(c,d,d),), CuCu2+-Zn-Zn2+ binarybinary system system (e,f), (e and,f), andCd -Zn Cd2+ binary-Zn2+ systembinary ( systemg,h). (g,h).
Heavy metals that displayed small hydration energies were easier to dehydrate and subsequently be adsorbed by the NaX. However, in multiple ion systems, those ions
MaterialsMaterials 20212021,, 1414,, x 4066 FOR PEER REVIEW 1312 of of 18 16
2.5 2.5 (a) (b) 2.0 2.0
1.5 1.5 Cu Pb Cu
1.0 Zn 1.0 Pb
Qe(mmol/g) Cd Qe(mmol/g)
0.0 0.0 0.0 0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0 0.00.51.01.52.02.53.03.54.0
C (mmol/L) C (mmol/L) 0 0 2.5 2.5 (c) (d) 2.0 Cu 2.0 Cd Zn 1.5 1.5 Cu Pb
Cd 1.0 1.0 Zn Qe(mmol/g) Qe(mmol/g) 0.5 0.5
0.0 0.0 0.0 0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0 0.0 0.5 1.0 1.5 2.0 2.5 3.0 3.5 4.0 C (mmol/L) C (mmol/L) 0 0 FigureFigure 5. 5. AdsorptionAdsorption capacity of NaX for heavy metalmetal ionsions presentpresent inin ternaryternaryand and quaternary quaternary systems: systems: ( a()a) Pb Pb2+2+-Cu-Cu2+2+-Zn2+, , 2+ 2+ 2+ 2+ 2+ 2+ 2+ 2+ 2+ 2+ ((bb)) Pb Pb2+-Cd-Cd2+-Cu-Cu,2+ (c,() cCd) Cd-Cu2+-Cu-Zn2+-Zn and2+ and(d) Pb (d)-Cd Pb2+-Cd-Cu2+-Zn-Cu2+. -Zn2+.
126.96.36.199. Mechanisms Mechanisms of of Selective Selective Adsorp Adsorptiontion of of Heavy Heavy Metal Metal Ions Ions by by NaX NaX NaX-Pb,NaX-Pb, NaX-Cd, NaX-Cd, NaX-Cu NaX-Cu and and NaX-Zn NaX-Zn re representpresent NaX NaX zeolite saturated with Pb2+, , CdCd2+2+, ,Cu Cu2+2+ andand Zn Zn2+,2+ respectively., respectively. The The infrared infrared spec spectratra and and pore pore size size distribution distribution of of NaX, NaX, NaX-Pb,NaX-Pb, NaX-Cd, NaX-Cd, NaX-Cu NaX-Cu and and NaX-Zn NaX-Zn zeolites zeolites are are presented presented in in Figure Figure 66a,b.a,b. The BETBET specificspeciﬁc surface surface area area (S (SBETBET) )and and the the pore pore parameters parameters of of NaX, NaX, NaX-Pb, NaX-Pb, NaX-Cd, NaX-Cd, NaX-Cu NaX-Cu andand NaX-Zn NaX-Zn zeolites zeolites are are presented presented in in Table Table 66.. AsAs shown shown in in Figure Figure 66a,a, thethe peakpeak atat 973973 cmcm−11 inin NaX NaX was was assigned assigned to to the the asymmetric asymmetric stretchingstretching vibration vibration of of Si-O-Si, Si-O-Si, Si-O-Al Si-O-Al and and O-Si-O groups, while the peakpeak atat 753753 cmcm−−1 correspondscorresponds to to the the symmetrical symmetrical stretching stretching vibration vibration of of the the Si-O-Si Si-O-Si or or Si-O-Al Si-O-Al groups groups . . TheThe peak peak located located at at 463 cm −1 1correspondscorresponds to to bending bending vibrations vibrations of of the the Si-O-Si Si-O-Si or or Si-O-Al Si-O-Al − − groupsgroups within within the the zeolite zeolite structur structure.e. Whereas, Whereas, the the peaks peaks at at 560 560 cm cm−1 and1 and 671 671 cm cm−1 may1 may be attributedbe attributed to vibration to vibration modes modes of ofthe the double double six-membered six-membered rings rings present present in in the the zeolite zeolite frameworkframework [16,37]. [16,37]. −1 NaX-PbNaX-Pb spectra spectra showed showed that that the peaks observed at 400–1000400–1000 cmcm−1 presentedpresented higher higher −1 −1 intensitiesintensities as as compared compared to those ofof thethe NaX.NaX. InIn addition,addition, peaks peaks at at 753 753 cm cm−1,, 560560 cmcm−1 andand −1 463463 cm cm−1 displayeddisplayed small small shifts. shifts. However, However, according according to to the the spectra, spectra, the the chemical chemical structure structure inin the the NaX-Cd NaX-Cd and and NaX-Zn NaX-Zn remained remained almost almost unchanged. unchanged. StructuralStructural changes changes of of the the NaX NaX after after adsorp adsorptiontion can can be be explained explained by by the the electronega- electroneg- tivityativity differences differences of of heavy heavy metal metal ions. ions. The The O O in in the the Si-O-Al Si-O-Al structure structure of of the the NaX NaX was was negativelynegatively charged.charged. TheThe greater greater the the electronegativity electronegativity of the of heavythe heavy metal ions,metal the ions, stronger the 2+ strongerthe ability the to ability attract to the attract electron the cloud electron of the cl oxygenoud of atomsthe oxygen in the atoms Si-O-Al. in Inthe NaX-Pb, Si-O-Al. Pb In NaX-Pb,displayed Pb a2+ stronger displayed oxygen a stronger binding oxygen capacity binding given capacity its higher given electronegativity its higher electronega- (2.33) as 2+ tivitycompared (2.33)to as those compared of Si(1.90) to those and of Al Si (1.61). (1.90) Therefore,and Al (1.61). Pb Therefore,reduced the Pb stability2+ reduced of the the
Materials 2021, 14, x FOR PEER REVIEW 14 of 18
stability of the Si-O-Al bonds and the double six-membered rings in the NaX framework. Similarly, the electronegativity of Cu (1.90), which was higher than that of Al (1.61), af- fected the stability of the Si-O-Al bonds within the NaX structure. The electronegativity of Cd (1.69) and Zn (1.65) were not bigger than that of Al (1.61), hence could not affect the structure of the NaX zeolite. Figure 6b shows the pore size distribution of NaX, NaX-Pb, NaX-Cd, NaX-Cu and NaX-Zn. It can be found that the pore size of NaX-Pb, NaX-Cd, NaX-Cu and NaX-Zn are bigger than that of NaX. This is due to a divalent ion exchange with two Na+. Therefore, the position is empty, making the pore size larger. The position of the main peak in pore size distribution is NaX-Pb > NaX-Cd > NaX-Cu > NaX-Zn, which corresponds to the adsorption capacity of four kinds of heavy metal ions and the exchanged Na+ position. Zn2+ cannot enter the β-cage and hexagonal cylindrical cage with small pore size. The Materials 2021, 14, 4066 adsorption capacity of Zn2+ is the smallest, thus, the change in pore size of NaX zeolite13 of 16is the least. The adsorption capacity of Pb2+ is the largest, and almost all the Na+ in NaX ze- olite can be exchanged. Therefore, the pore size of NaX-Pb is the largest. Si-O-AlCompared bonds and with the NaX, double the six-membered t-plot micropore rings surface in the area NaX and framework. total pore Similarly, volume the of electronegativityNaX-Pb, NaX-Cd, of NaX-Cu, Cu (1.90), NaX-Zn which wasreduced higher significantly than that of (Table Al (1.61), 6). For affected Pb and the Cu stability with ofhigher the Si-O-Al electronegativity, bonds within the the pore NaX volume structure. and The micropore electronegativity surface area of Cd of (1.69)NaX-Pb and and Zn (1.65)NaX-Cu were decreased not bigger more. than The that ions of Alwith (1.61), high hence electronegativity could not affect were the more structure likely to of theun- NaXdergo zeolite. acid-base coordination and hydrolysis, thus occupying pore volume.
(a) 973 (b) 463 753 560 NaX－Zn NaX－Pb NaX－Cu
NaX－Cu NaX－Cd NaX－Cd NaX－Pb NaX－Zn
1000 900 800 700 600 500 400 0.56 0.57 0.58 0.59 Wavenumber (cm-1) Pore size (nm) Figure 6. Infrared spectra ((a)) andand porepore sizesize distributiondistribution ((bb)) ofof NaX,NaX, NaX-Pb,NaX-Pb, NaX-Cd,NaX-Cd, NaX-CuNaX-Cu andand NaX-Zn.NaX-Zn.
Table 6. The BET speciﬁc surface area (SBET) and pore parameters of NaX, NaX-Pb, NaX-Cd, NaX-Cu and NaX-Zn zeolites.
Average t-Plot Micropore Total Pore S (m2/g) Pore Size (nm) BET Surface Area (m2/g) Volume (cm3/g) NaX 0.556 712.7 701.9 0.3556 NaX-Pb 0.599 351.9 346.2 0.1716 NaX-Cd 0.611 551.3 545.8 0.2720 NaX-Cu 0.613 515.9 484.9 0.2467 NaX-Zn 0.611 592.2 578.8 0.2910
Figure6b shows the pore size distribution of NaX, NaX-Pb, NaX-Cd, NaX-Cu and NaX-Zn. It can be found that the pore size of NaX-Pb, NaX-Cd, NaX-Cu and NaX-Zn are bigger than that of NaX. This is due to a divalent ion exchange with two Na+. Therefore, the position is empty, making the pore size larger. The position of the main peak in pore size distribution is NaX-Pb > NaX-Cd > NaX-Cu > NaX-Zn, which corresponds to the adsorption capacity of four kinds of heavy metal ions and the exchanged Na+ position. Zn2+ cannot enter the β-cage and hexagonal cylindrical cage with small pore size. The adsorption capacity of Zn2+ is the smallest, thus, the change in pore size of NaX zeolite is the least. The adsorption capacity of Pb2+ is the largest, and almost all the Na+ in NaX zeolite can be exchanged. Therefore, the pore size of NaX-Pb is the largest. Compared with NaX, the t-plot micropore surface area and total pore volume of NaX-Pb, NaX-Cd, NaX-Cu, NaX-Zn reduced signiﬁcantly (Table6). For Pb and Cu with higher electronegativity, the pore volume and micropore surface area of NaX-Pb and NaX- Cu decreased more. The ions with high electronegativity were more likely to undergo acid-base coordination and hydrolysis, thus occupying pore volume. Materials 2021, 14, x FOR PEER REVIEW 15 of 18
Table 6. The BET specific surface area (SBET) and pore parameters of NaX, NaX-Pb, NaX-Cd, NaX-Cu and NaX-Zn zeolites.
Average t-Plot Micropore Total Pore SBET (m2/g) Pore Size(nm) Surface Area (m2/g) Volume (cm3/g) NaX 0.556 712.7 701.9 0.3556 NaX-Pb 0.599 351.9 346.2 0.1716 NaX-Cd 0.611 551.3 545.8 0.2720 NaX-Cu 0.613 515.9 484.9 0.2467 Materials 2021, 14, 4066 NaX-Zn 0.611 592.2 578.8 0.2910 14 of 16
The selectivity of NaX was related to the hydration energy and electronegativity of the adsorbed metal ions, which are relevant to the pore size and skeleton negative The selectivity of NaX was related to the hydration energy and electronegativity of charge of the NaX. The supercage pore diameter of the NaX zeolite was 0.74–0.78 nm, the adsorbed metal ions, which are relevant to the pore size and skeleton negative charge andof the that NaX. of Thethe 6-membered supercage pore rings diameter was 0.28 of the nm NaX (Figure zeolite 7a), was and 0.74–0.78 the diameter nm, and of that the of hydratedthe 6-membered heavy metal rings ions was 0.28was nmlarger (Figure than7 thesea), and values. the diameter Therefore, of the dehydrated hydrated heavy metalmetal ions ions may was largerenter thanthe supercage these values. pores Therefore, and partially dehydrated enter heavythe 6-membered metal ions may rings enter in thethe supercageadsorption pores process. and partiallyThe oxygen enter theskeleton 6-membered present rings in inthe the aluminized adsorption oxygen process. tetrahedron structure [AlO4] of the NaX which is also known as its structural base center The oxygen skeleton present in the aluminized oxygen tetrahedron structure [AlO4] of the isNaX negatively which ischarged also known (Figure as 7b). its structural According base to the center Lewis is negativelyacid-base theory, charged heavy (Figure metal7b). ionsAccording are acidic to the and Lewis are able acid-base to receive theory, electrons heavy metal . ionsTherefore, are acidic they and can are form able acid-base to receive coordinatedelectrons [38 structures]. Therefore, with they the can O form present acid-base in the coordinated base center structures of NaX with(Figure the O7c). present The higherin the basethe electronegativity center of NaX (Figure of the7 c).heavy The highermetal ions, the electronegativity the stronger their of ability the heavy to attract metal theions, electron the stronger clouds their of negatively ability to charged attract the oxygen electron and, clouds the stronger of negatively the coordinate charged oxygenbonds formedand, the with stronger O. Therefore, the coordinate in multi-component bonds formed withsystems, O. Therefore, heavy metal in multi-componentions with small hydrationsystems, heavyenergy metal may ionsenter with the smallpores hydrationof NaX, but energy with maythe adsorption enter the pores sites ofin NaX,the NaX but thatwith can the be adsorption equally occupied sites in the by NaX different thatcan heavy beequally metal ions, occupied their byelectronegativity different heavy is metal the keyions, to theirdetermine electronegativity their selective is the adsorption. key to determine their selective adsorption.
FigureFigure 7. 7. DiagramDiagram of of the the NaX NaX zeolite framework ((aa),), skeletonskeleton negatively negatively charged charged of of [AlO [AlO4](4]b ()b and) and acid-base acid-base coordination coordination (c). (c). 4. Conclusions Due to the restricted interaction of the hydration diameter of the heavy metal ions and the pore size of the NaX, the maximum adsorption capacity in single system for Pb2+, Cd2+, 2+ 2+ Cu and Zn was 2.38 mmol/g, 2.14 mmol/g, 1.87 mmol/g, and 1.68 mmol/g, respec- tively. Heavy metal ions with relatively low hydration energy were easier to dehydrate before entering the NaX pore, and possessed higher adsorption capacity. The selective adsorption between two heavy metal ions resulted in an introduction of separation factor α and the afﬁnity constant KEL from the extended Langmuir isothermal model. The selective adsorption capacity and afﬁnity followed the order of Pb2+ > Cd2+ ≈ Cu2+ > Zn2+, implying Pb2+ was the most favorable species and the afﬁnity toward Zn2+ was the weakest. The separation factor achieved was about 1, implying the selectivity of NaX towards Cu2+ and Cd2+ was similar. Desorption of the metal ions with low electronegativity in binary solute was observed in the kinetic section and the possible mechanism could be described as Materials 2021, 14, 4066 15 of 16
direct displacement effect. The direct displacement mechanism of the adsorption process might prove that the electronegativity of metal ions should be a key factor associated with the selective adsorption on the NaX. The higher the electronegativity of the heavy metal ions, the stronger their ability to attract the electron clouds of negatively charged oxygen present in the NaX frameworks.
Author Contributions: H.L., X.F., E.A. and D.R. conceived and designed the methodology; X.F. and E.A. performed the experiment and prepared the composite materials; H.L. and D.R. analyzed the data. All authors evaluated and discussed the results, and wrote the paper together. All authors have read and agreed to the published version of the manuscript. Funding: Wuhan Science and Technology Planning Project (Grant No 2020020601012274). Institutional Review Board Statement: Not applicable. Informed Consent Statement: Not applicable. Data Availability Statement: All relevant data presented in the article are stored according to institutional requirements and as such are not available online. However, all data used in this manuscript can be made available upon request to the authors. Acknowledgments: Greater thanks goes to the Open Fund of Hubei Key Laboratory for Efﬁcient Utilization and Agglomeration of Metallurgic Mineral Resources from Wuhan University of Science and Technology (2017zy008). Conﬂicts of Interest: The authors declare no conﬂict of interest.
References 1. Corda, N.; Kini, M.S. Recent studies in adsorption of Pb(II), Zn(II) and Co(II) using conventional and modiﬁed materials: A review. Sep. Sci. Technol. 2019, 55, 2679–2698. [CrossRef] 2. Hong, M.; Yu, L.; Wang, Y.; Zhang, J.; Chen, Z.; Dong, L.; Zan, Q.; Li, R. Heavy metal adsorption with zeolites: The role of hierarchical pore architecture. Chem. Eng. J. 2019, 359, 363–372. [CrossRef] 3. Burakov, A.E.; Galunin, E.V.; Burakova, I.V.; Kucherova, A.E.; Agarwal, S.; Tkachev, A.G.; Gupta, V.K. Adsorption of heavy metals on conventional and nanostructured materials for wastewater treatment purposes: A review. Ecotoxicol. Envrion. Saf. 2018, 148, 702–712. [CrossRef][PubMed] 4. Ghaffari, A.; Tehrani, M.S.; Husain, S.W.; Anbia, M.; Azar, P.A. Adsorption of chlorophenols from aqueous solution over amino-modiﬁed ordered nanoporous silica materials. J. Nanostructure Chem. 2014, 4, 1–10. [CrossRef] 5. Skwarek, E.; Janusz, W. Adsorption of Cd(II) ions at the hydroxyapatite/electrolyte solution interface. Sep. Sci. Technol. 2015, 51, 11–21. [CrossRef] 6. Kolodynska, D.; Skwarek, E.; Hubicki, Z.; Janusz, W. Effect of adsorption of Pb(II) and Cd(II) ions in the presence of EDTA on the characteristics of electrical double layers at the ion exchanger/NaCl electrolyte solution interface. J. Colloid Interface Sci. 2009, 333, 448–456. [CrossRef][PubMed] 7. Bhattacharyya, K.G.; Gupta, S.S. Adsorption of a few heavy metals on natural and modiﬁed kaolinite and montmorillonite: A review. Adv. Colloid Interface Sci. 2008, 140, 114–131. [CrossRef][PubMed] 8. Padilla-Ortega, E.; Leyva-Ramos, R.; Flores-Cano, J.V. Binary adsorption of heavy metals from aqueous solution onto natural clays. Chem. Eng. J. 2013, 225, 535–546. [CrossRef] 9. Ghasemi, Z.; Sourinejad, I.; Kazemian, H.; Rohani, S. Application of zeolites in aquaculture industry: A review. Rev. Aquac. 2018, 10, 75–95. [CrossRef] 10. Purna Chandra Rao, G.; Satyaveni, S.; Ramesh, A.; Seshaiah, K.; Murthy, K.S.; Choudary, N.V. Sorption of cadmium and zinc from aqueous solutions by zeolite 4A, zeolite 13X and bentonite. J. Environ. Manag. 2006, 81, 265–272. [CrossRef][PubMed] 11. Ismail, A.A.; Mohamed, R.M.; Ibrahim, I.A.; Kini, G.; Koopman, B. Synthesis, optimization and characterization of zeolite A and its ion-exchange properties. Colloids Surf. A Physicochem. Eng. Asp. 2010, 366, 80–87. [CrossRef] 12. Yuna, Z. Review of the natural, modiﬁed, and synthetic zeolites for heavy metals removal from wastewater. Environ. Eng. Sci. 2016, 33, 443–454. [CrossRef] 13. Ahmed, I.A.M.; Young, S.D.; Mosselmans, J.F.W.; Crout, N.M.J.; Bailey, E.H. Coordination of Cd2+ ions in the internal pore system of zeolite-X A combined EXAFS and isotopic exchange study. Geochim. Et Cosmochim. Acta 2009, 73, 1577–1587. [CrossRef] 14. Song, H.; Cheng, H.; Zhang, Z.; Cheng, F. Adsorption properties of zeolites synthesized from coalﬂy ash for Cu(II). J. Environ. Biol. 2014, 35, 983–988. 15. Mohamed, R.M.; Ismail, A.A.; Kini, G.; Ibrahim, I.A.; Koopman, B. Synthesis of highly ordered cubic zeolite A and its ion-exchange behavior. Colloids Surf. A Physicochem. Eng. Asp. 2009, 348, 87–92. [CrossRef] Materials 2021, 14, 4066 16 of 16
16. Nibou, D.; Mekatel, H.; Amokrane, S.; Barkat, M.; Trari, M. Adsorption of Zn2+ ions onto NaA and NaX zeolites: Kinetic, equilibrium and thermodynamic studies. J. Hazard. Mater. 2010, 173, 637–646. [CrossRef][PubMed] 17. Mekatel, H.; Amokrane, S.; Benturki, A.; Nibou, D. Treatment of polluted aqueous solutions by Ni2+, Pb2+, Zn2+, Cr6+,Cd2+ and Co2+ ions by ion exchange process using faujasite zeolite. Procedia Eng. 2012, 33, 52–57. [CrossRef] 18. Ziyath, A.M.; Mahbub, P.; Goonetilleke, A.; Adebajo, M.O.; Kokot, S.; Oloyede, A. Inﬂuence of physical and chemical parameters on the treatment of heavy metals in polluted stormwater using zeolite—A Review. J. Water Resour. Prot. 2011, 3, 758–767. [CrossRef] 19. Izidoro, J.D.C.; Fungaro, D.A.; Abbott, J.E.; Wang, S. Synthesis of zeolites X and A from ﬂy ashes for cadmium and zinc removal from aqueous solutions in single and binary ion systems. Fuel 2013, 103, 827–834. [CrossRef] 20. Hui, K.S.; Chao, C.Y.; Kot, S.C. Removal of mixed heavy metal ions in wastewater by zeolite 4A and residual products from recycled coal ﬂy ash. J. Hazard. Mater. 2005, 127, 89–101. [CrossRef][PubMed] 21. Visa, M. Synthesis and characterization of new zeolite materials obtained from ﬂy ash for heavy metals removal in advanced wastewater treatment. Powder Technol. 2016, 294, 338–347. [CrossRef] 22. Heo, N.H.; Sung, S.W.J.; Park, W.; Park, M.; Lim, W.T. Crystal structures of fully indium-exchanged Zeolite X. Am. Chem. Soc. 2000, 104, 8372–8381. [CrossRef] 23. Takaishi, T. Ordered distribution of Na ions in dehydrated NaX zeolite. Zeolites 1996, 17, 389–392. [CrossRef] 24. Notker, R.; Georgi, N.V.; Konstantin, M.N. Density functional model cluster studies of metal cations, atoms, complexes, and clusters in zeolites. In Host-Guest-Systems Based on Nanoporous Crystals; Wiley Online Library: Hoboken, NJ, USA, 2003; pp. 339–357. ISBN 3-527-30501-7. 25. Zanin, E.; Scapinello, J.; de Oliveira, M.; Rambo, C.L.; Franscescon, F.; Freitas, L.; de Mello, J.M.M.; Fiori, M.A.; Oliveira, J.V.; Dal Magro, J. Adsorption of heavy metals from wastewater graphic industry using clinoptilolite zeolite as adsorbent. Process. Saf. Environ. Prot. 2017, 105, 194–200. [CrossRef] 26. Nightingale, E.R. Phenomenological theory of ion solvation: Effective radii of hydrated ions. J. Phys. Chem. 1959, 63, 1381–1387. [CrossRef] 27. Teppen, B.J.; Miller, D.M. Hydration energy determines isovalent cation exchange selectivity by clay minerals. Soil Sci. Soc. Am. J. 2006, 70, 31–40. [CrossRef] 28. Ning, C.; Xu, M.; Hui, D.C.W.; Lin, C.S.K.; McKay, G. Study of quench effect on heavy metal uptake efﬁciency by an aluminosilicate- based material. Chem. Eng. J. 2017, 311, 37–45. [CrossRef] 29. Xu, M.; Hadi, P.; Ning, C.; Barford, J.; An, K.J.; McKay, G. Aluminosilicate-based adsorbent in equimolar and non-equimolar binary-component heavy metal removal systems. Water Sci. Technol. 2015, 72, 2166–2178. [CrossRef] 30. Selim, A.Q.; Sellaoui, L.; Ahmed, S.A.; Mobarak, M.; Mohamed, E.A.; Lamine, A.B.; Erto, A.; Bonilla-Petriciolet, A.; Seliem, M.K. Statistical physics-based analysis of the adsorption of Cu2+ and Zn2+ onto synthetic cancrinite in single-compound and binary systems. J. Environ. Chem. Eng. 2019, 7, 103217. [CrossRef] 31. Li, L.; Liu, F.; Jing, X.; Ling, P.; Li, A. Displacement mechanism of binary competitive adsorption for aqueous divalent metal ions onto a novel IDA-chelating resin: Isotherm and kinetic modeling. Water Res. 2011, 45, 1177–1188. [CrossRef] 32. Sheng, P.X.; Ting, Y.P.; Chen, J.P. Biosorption of heavy metal ions (Pb, Cu, and Cd) from aqueous solutions by the marine alga sargassum sp. in single- and multiple-metal systems. Am. Chem. Soc. 2007, 46, 2438–2444. [CrossRef] 33. Girish, C.R. Various isotherm models for multicomponent adsorption a review. Int. J. Civ. Eng. Technol. 2017, 8, 80–86. 34. Zhang, X.P.; Liu, F.Q.; Zhu, C.Q.; Xu, C.; Chen, D.; Wei, M.M.; Liu, J.; Li, C.H.; Ling, C.; Li, A.M.; et al. A novel tetraethylene- pentamine functionalized polymeric adsorbent for enhanced removal and selective recovery of heavy metal ions from saline solutions. RSC Adv. 2015, 5, 75985–75997. [CrossRef] 35. Liu, X.J.; Zhu, Y.X.; Gao, F. Inorganic Elemental Chemistry; Science Press: Beijing, China, 2010. (In Chinese) 36. Liu, C.C.; Wang, M.K.; Chiou, C.S.; Li, Y.S.; Yang, C.Y.; Lin, Y.A. Biosorption of chromium, copper and zinc by wine-processing waste sludge: Single and multi-component system study. J. Hazard. Mater. 2009, 171, 386–392. [CrossRef] 37. Zavareh, S.; Farrokhzad, Z.; Darvishi, F. Modiﬁcation of zeolite 4A for use as an adsorbent for glyphosate and as an antibacterial agent for water. Ecotoxicol. Environ. Saf. 2018, 155, 1–8. [CrossRef][PubMed] 38. Pearson, R.G. Physical and inorganic chemistry. J. Am. Chem. Soc. 1963, 85, 3533–3539. [CrossRef]